UNIVERSITA’ DEGLI STUDI DI PARMA
Dottorato di ricerca in Scienze Chimiche Ciclo XXIII (2008-2010)
Wood treatments with siloxane materials and metal complexes
for preservation purposes
Prof. Alberto Girlando Tutor:
Prof. Giovanni Predieri
1.1 Preface: wood degradation and preservatives 1.2 Wood structure and properties
1.2.1 Wood structure 1.2.2 Wood properties 1.3 Wood degradation
1.3.1 Abiotic degradation 1.3.2 Biotic degradation
188.8.131.52 Fungi 184.108.40.206 Insects
220.127.116.11 Wood durability against fungi and insects
1.4 Treatments for the improvement of wood properties
1.4.1 Surface Coatings and penetrating treatments 1.4.2 Modification of wood
18.104.22.168 Modification with alkoxysilanes 1.5 Preservation of wood from biotic decay
1.5.1 Remedial treatments 1.5.2 Preventive treatments
1.5.3 Modification of wood by sol-gel process for preservative purpose
1.5.4 Elements involved as active principles in inorganic biocides permitted till now
1.6 Aim of the work
Page 9 9 11 11 22 24 24 27 28 32
34 35 35 36 39
41 41 43
2.1 Materials and analytical instruments
2.1.1. Starting chemicals and analytical instruments 2.1.2. Wood samples features
2.2 Preparations of the preservative formulations
2.2.1. TEOS-APTES formulations
2.2.2. TEOS-APTES-COPPER formulations
2.2.3. SODIUM METASILICATE-COPPER formulation 2.2.4. TEOS-COPPER formulations
2.2.5. TEOS-APTES-BORON formulations
2.2.6. Commercial colloidal SiO2-boron formulations 2.2.7. TEOS formulations with silver nanoparticles 2.2.8. Polyaminoamide(PAA) formulations
2.2.9. Copper glycinate in acqueous solutions 2.2.10.Metal salicylates in linseed oil solutions 2.1.11 Metal salicylates in ethylene glycol 2.3. Wood samples treatment
2.3.1 Samples preparation 2.3.2 Methods of wood treatment
22.214.171.124 Application by immersion 126.96.36.199 Application by impregnation 2.4. Characterization of the treated wood
2.4.1 Weight characterization 2.4.2 Analytical characterization 2.4.3 Leaching tests
2.5. Efficacy tests against biological attack
62 62 63 64 65 66 67 67 68 68 73 77 78 78 78 78 79 83 83 83 87 88
2.5.1 Efficacy of sol-gel treatments against brown rot and white rot fungi
2.5.2 Efficacy of sol-gel treatments against termites - no- choice test
2.5.3 Efficacy of copper glycinate formulations against the brown rot fungus Coniophora puteana
2.5.4 Efficacy of copper and zinc salicylate formulations in linseed oil against termites
2.5.5 Efficacy of copper and zinc salicylate formulations in ethylene glycol against termites
2.6 Physico-mechanical characterization of treated specimens
2.6.1 Colorimetric measurements 2.6.2 Sorption test
2.6.3 Dimensional stability
3. Results and Discussion
PART A - TREATMENTS WITH SILOXANE SOL-GEL MATERIALS 3.1. Characterization of treated wood
3.1.1 Sol-gel treatments with addiction of copper 3.1.2 Sol-gel treatments with addiction of boron
3.1.3 Further hybrid inhorganic-organic treatments with addiction of zinc or silver
3.2. Evaluation of preservative effectiveness
3.2.1 Effectiveness of sol-gel treatments coupled with copper and boron against subterranean termites
3.2.2 Effectiveness of sol-gel treatments against fungi basdiomycetes
97 98 101
104 111 134
PART B - STUDIES ON PRESERVATIVES BASED ON METAL CHELATES
3.3. Copper glycinate formulations: evaluation of preservative properties against the brown rot fungus C.puteana
3.4. Wood treatment with metal complexes in linseed oil and ethylene glycol
3.4.1 Zinc-salicylate formulation 3.4.2 Copper-salicylate formulation
3.4.3 Salicylates effiectiveness against termites PART C – PHYSICAL-MECHANICAL CHARACTERIZATIONS
3.5. Physical and mechanical properties of wood treated samples
3.5.1 Colorimetric characterization
3.5.2 Sorption and dimensional stability tests
5. References 6. Aknowledgments
155 155 159 161
168 168 171
1.1 Preface: wood degradation and preservatives
Wood has been conveniently used as material for a large variety of human artifacts throughout the course of history: architectural woodworks (especially beams, flooring, roofs, ceiling), frames, outdoor or indoor furniture, ship building, railway sleepers and siding, exterior joinery, carpentry, pilings, panelling, tool handles and cutlery, musical instruments or sport equipments. It has also had great importance in the past in the artistic field and it has long been used for paintings on board, sculptures, carvings and church furniture such as altars and choirs. (Italy in particular has got great wooden artistic and historical heritage).
Wood is also widely used nowadays especially in the building and construction industries, both thanks to its many technical advantages such as high tensile strength, high elastic modulus, low density and insulation properties, and thanks to its revolving nature, low cost and aesthetic features.
Its principal disadvantageous characteristics are due to its organic constitution: it is slowly destroyed by the long-term impact of oxygen, light and water under atmospheric conditions; unprotected wood will eventually warp, split, rot and decay from water absorption, and also grey by UV exposure. Moreover, wood is a source of nutrients for micro-organisms, fungi and insects, leading to its complete biological destruction (Eaton, 1993).
Therefore, a lot of treatments have been essayed on wood in the past trying to overcome these drawbacks and to enhance wood durability, hydrophobicity, dimensional stability, strength and hardness, weathering performance and flame resistance. Among them, a large variety of compounds has been tested for wood modification, including anhydrides, carboxylic acids, isocyanates, aldehydes, alkyl chlorides, lactones, nitriles, and epoxides (Rowell 1983; Militz et al. 1997; Norimoto 2001).
As regards the improvement of durability against biological (biotic decay) agents, most of the preservative products developed in the chemical industry in the19th century have been recently banned by European Union because of their high toxicity to human. They were mainly polychlorine and phenolic compounds or arsenic or chrome salts and/or
copper salts, easily leachable and diffusible in the environment.
Research has been focused on developing new non-toxic and eco-friendly wood preservatives, eventually endowed of additional properties for increasing wood mechanical characteristics, dimensional stability, flame or UV resistance.
This thesis deals with the development of new wood treatments for increasing fungal and termite decay resistance.
The treatments performed are based on the well known antifungal and insect-deterrent activities of Cu, Zn and Ag, with the aim of reducing their environmental impact by means of an adequate fixation to wood, reached through two different ways:
1. impregnation of wood with Cu and Zn metal complexes soluble in water or organic solvents;
2. modification of wood with inorganic or inorganic-organic hybrid siloxane materials incorporating the metals or anchoring them through coordinative linkages.
Treatments based on the combined action of the above mentioned compounds with boric acid, used since the 1930’s for protection of timber from biological attack, have also been performed, to improve preservation efficacy of the new formulations and to study their capability to increase boron fixation to wood.
Various methods of treatment, ranging from immersion to impregnation under vacuum, have been performed. For each treatment interaction and diffusion into the wood structure, preservative efficacy against fungi and/or termites and improvement of other chemical or physical properties have been evaluated.
1.2 Wood structure and properties
Wood is a natural organic composite material, that used for human artefacts being almost all obtained from the stem of plants belonging to the Spermatophyta subdivisions of gymnosperms (known as conifers) and angiosperms (deciduous trees). The term softwood is used to describe wood from conifers, and it is opposed to hardwood, which is the wood from angiosperm trees (Nardi, 2006).
1.2.1 Wood structure
Wood structure can be examined at different levels (Figure 1):
1) Stem macro structure 2) Timber microscopic structure 3) Cellular structure
4) Wood cell ultrastructure and wall chemistry
Figure 1 Different levels of examination of the wood structure
2) timber structure 3) cellular structure
4) wood cell ultrastructure
1) Stem macro structure
Looking at the cross section of a tree stem, several distinctive parts are visible (Figure 2). From the outside to pith, we can distinguish:
- the cork, i.e. the outermost physiologically dead layer of a woody stem, whose main functions are the protection against damage from parasites, herbivorous animals and diseases (dehydration and fire) and the control gas exchange.
- the phloem, i.e. the live vascular tissue with the role of conduction of sugars and other dissolved foods (lymph) produced by the leaves. It is discarded in the production of wooden items;
- the vascular cambium, i.e. the tissue responsible for the secondary growth of stems and roots (secondary growth occurs after the first season and results in increase in thickness); it produces phloem cells toward the outside and xylem cells toward the central axis of the stem.
Figure 2 Stem structure
Figure 2 Scheme of the stransversal section of a stem, showing the distinctive parts of its macro structure.
All the tissues comprised between the cambium and the stem central axis are called “wood”.
alburno annual rings
cork vascular cambium
All the tissues comprised between the cambium and the stem central axe are called
“wood”. In a plant cross-section wood shows growth rings, that in the temperate species correspond to the annual activity of the cambium and are due to the alternate production of cells with large lumen (“spring wood”) and cells shorter with thicker walls (“summer wood" or "latewood"). Medullary rays, perpendicular to the growth rings and allowing the radial transmission of sap and storing up the reserves of carbohydrates and mineral salts, are also visible in a lot of tree species.
As the tree stem increases in circumference, the central part begins to lose water and stored food substances. The central zone of the stem becomes infiltrated with oils, gums, resins, tannins and aromatic compounds and when the transformation is complete these cells eventually die.
So we can distinguish:
- sapwood (alburno): it is the younger, outermost wood and it is its functional and active region: in the growing tree its principal functions are to conduct water from the roots to the leaves and to store up the reserves;
- heartwood (duramen): it’s the stem central area, it is formed by dead cells whose function is no longer of conduction but only of mechanical support to the stem.
The genetically programmed process of sapwood transformation in heartwood is known as“duramification”. In many species, heartwood exhibits an intensification of colour because of oxidation of phenolic compounds in the deposited substances. Thus this region often appears darker, but in some species e.g. aspen, beech and sycamore, the colour difference between sapwood and heartwood is negligibile. Heartwood has the same strenght as sapwood but has greater natural resistance to biological attack because of toxic compounds mostly deposited in the cells during its formation and also because of its lower permeabiliy to water and oxygen.
Chemical preservative treatments are performed on alburno rather than on duramen because of its lower natural durability and higher impregnation properties.
2) Timber structure
Wood has a porous, heterogeneous and anisotropic structure. For this reason, three different wood sections, called “reference planes of wood” (transverse (Tr), tangential (Tg) and radial (Ra) section), are necessary for a complete characterization (Figure 3).
They correspond to cuts made in the three different directions of wood anisotropy (longitudinal (L), radial (R) and tangential (T)).
Figure 3 Wood reference planes and directions of anisotropy. Tr = transverse section; Tg= tangential section; Ra=radial section; L=longitudinal axis; R = radial axis; T=tangential axis.
All commercially relevant tree species (excluding monocotyledonous species such as palms) are either hardwoods or softwoods.Softwood, called omoxilo, consists for the 90 to 95% by volume of tracheids, having both the functions of raw sap conduction and support: they consist of dead cells with tangential diameter of about 70 µm and radial diameter variable depending on their position in the annual ring. Softwood also consists of axial and ray parenchyma cells, storing carboyhidrates and mineral salts.
Hardwood is called eteroxilo because of the difference, even qualitative, between vessels, with the functions of raw sap cpnduction, and fibers, responsible for mechanical resistance. Vessels are formed by dead cylindrical cells with diameter ranging from 25 to 500 µm or even more, arranged in axial columns without any wall separation; fibers are formed by elongated, thick-walled, lignified dead cells. Parenchyma and epithelial cells are also present.
Differences between hardwood and softwood are mainly visible in transversal section.
Resinous canals in softwood are often noticeable at naked eye. Pores corresponding to the vessels in hardwood are sometimes even visible. Microscopic observations of the three wood reference sections enable to distinguish among different ligneous species, taking attention to some features such as:
- presence of resinous canals and their morphology (lumen diameter, cell-wall thickness) (softwood)
- vessels dimension and distribution (hardwood) - axial parenchyma distribution
- more ore less continuity between latewood and spring wood in annual rings - presence of radial tracheids (softwood)
- characteristics of pits, that connect adjacent ray cells and contiguous axial and ray cells
- ray parenchyma dimensions and distribution and ray parenchyma cells morphology (Figure 4).
Radia l section
Radial s ection Tangential section
Transversal section Transversal section
Figure 4 Schematic representation of wood. Softwood: 1. tracheids, 2. ray parenchyma, 3. resinous canals. Hardwood: 1. latewood: 2. spring wood, 3. ray parenchyma, 4. vessels, 5 axial parenchyma (from www.sfera-group.it).
3) The cell wall Structure
Every wood tissue is composed by cells, each formed by the cell wall and by the internal cell lumen. Whereas the lumen is a cavity, the cell wall has a complex structure. It is composed of several layers synthesized at different times in the cell differentiation process. Moving from the lumen (Figure 5), we can distinguish:
- the secondary wall - the primary wall - the middle lamella.
Figure 5 Schematic representation of the cell wall structure, showing the primary wall and the secondary wall with its different sub-layers (S1, S2, S3). Middle lamella is also represented among adjacent cells (from Nardi, 2006).
The secondary wall has a thickness of about 0,1mm and it is mainly composed of cellulose. Cellulose microfibrils are aligned parallel to each other and arranged in three sub-layers (S1, S2 and S3) with different microfibril orientation. These layers can also contain lignin, hemicellulose and pectic substances. The primary wall, with thickness of 0.5 to 1.5 µm, is mainly composed of pectine and lignin. The middle lamella constitutes the cementing layer between adjacent cells, is amorphous in character, is more or less devoid of cellulose but is rich in pectin compounds and especially in lignin (70%).
4) Wood cell ultrastructure and wall chemistry
The major chemical components in wood cell walls are: cellulose (between 40 to 55% of the total cell wall mass), hemicellulose (approximately 25-40%) and lignin (18-33%).
Proteins (<10 %) and compounds of lower molecular weight (extractable, mineral salts) (<1 %) can also be present.
Cellulose exists in the form of microfibrils whose function is to impart tensile strength to the cell wall; hemicellulose plays the role of a matrix material; lignin is present as an encrusting substance and contributes to impart compressive strength.
Figure 6 Scheme of cellulose structure.
Among the polysaccharides, cellulose is a linear polymer formed by the sequence of monosaccharide units of D-anhydroglucopyranose linked by β 1-O-4 glycosidic bonds
(Figure 6). As a polymer, Cellulose can be described as the repetition of the basic structure of the disaccharide cellobiose (1.03 nm in length). The degree of polymerization (the number of glucose units per cellulose molecule) in wood ranges between 8000 and 10000, depending on the tree specie (Campanella, 2007).
The glycosidic bonds are formed through the reaction between the hydroxyl group of a glucuose molecole and the carbonylic group (aldehydic or chetonic) of another glucose molecule. The C(1)-OH group is oriented over the median plane of the pyranosic ring (β- glycosidic link), conferring linearity to the cellulose chain and promoting the formation of intrachain hydrogen bonds among the singular glycosidic units.
Interchain hydrogen bonds between the oxyidrilic groups of adjacent chains cause the highly ordered arrangement of molecular chains in microfibrils and fibrils. Cellulose I and cellulose II differ for the parallel (cellulose I) or anti-parallel (cellulose II) orientation between adjacent chains (Nardi,2006).
As stated by the current model of microfibril organization, crystalline regions take place, characterized by monocline symmetry (in the case of cellulose I). They take turns with amorphous regions.
The higher is the order degree, the lower is water penetration. The non-crystalline zones also absorb more water than the crystalline ones because of the presence of more –OH groups free from intermolecular linkages.
Hemicellulose represent a class of non-cellulosic polysaccharides. They are relatively short, branched heteropolymers, whose monosaccharide components are D-glucose, D- xylose (often acetylated in position 2 or 3), L-ramnose, D-mannose, L-arabinose, D- galactose as well as the uronic acid of glucose and galactose, depending mainly on the tree specie, the wood tissue and cell wall layer. For example, the middle lamella exhibits a relatively even balance of monosaccharide components in both hardwoods and softwoods, whereas the composition of the secondary wall layers shows a preponderance of xylan components in hardwood and glucomannan components in softwood.
The monosaccharide units are linked by 1-3, 1-6 and 1-4 glycosidic bonds, to form polymers having a degree of polymerization usually lower than 200 (Figure 7).
Figure 7 Schematic representation of hemicellulose 1-4 glycosidic bonds between adjacent monosachharides (from Campanella, 2007).
Due to the chain length, to the presence of ramifications and to the non-crystalline structure, hemicelluloses are more soluble in water than cellulose.
In addition, they are enough soluble in alkali because of the presence of carboxylic groups; they are more reactive than cellulose and more easily attacked by micro- organisms.
Lignin is a complex aromatic three-dimensional polymer of phenylpropenic alcohols and is completely amorphous. It presents different structure depending on the vegetal specie and kind of wood. There are three types of phenylpropenic alcohols from which all lignins are constructed: p-coumaryl alcohol [4-(3-hydroxy-1-propenyl)phenol], coniferyl alcohol [4-(3-hydroxypropenyl)-2-methoxyphenol] and sinapyl alcohol [4-(3- hydroxypropenyl)- 2,6-dimethoxy-phenol]. The major difference in the chemical structure of these monomers is the presence or absence of methoxyl (-OCH3) groups at the 3 and 5 positions of the aromatic ring (Figure 8).
Figure 8 Phenylpropenic alcohols of lignins: (1) paracoumaryl alcohol, (2) coniferyl alcohol (3) sinapyl alcohol.
Upon incorporation into lignin, they are referred to as syringyl (S), guaiacyl (G), or hydroxyphenyl (H) units, respectively.
The dehydrogenation of these alcohols, due to the laccase and peroxidase enzymes of the plants, leads to the formation of the mesomeric forms of the phenoxy radicals, that polymerize by radical coupling forming lignin. In this way the phenylpropenic units result linked through C-O-C or C-C linkages, forming polymers with high molecular weight (from 2000 to 15000 a.m.u.) (Figure 9).
Several models have been proposed to explain the structure of hardwood and softwood lignin. It is now generally accepted that softwood lignin is formed mainly from the dehydrogenative polymerization of conyferyl alchol, that hardwood lignin is derived from the dehyrogenative polymerization of coniferyl and sinapyl alcohols and that grass lignin is derived from the dehydrogenative polymerization of coniferyl, sinapyl and p-coumaril alcohols (Higuchi, 1985).
Over 70% of the total lignin occurs in the secondary wall of early wood cells and over 80%
in latewood cells. The lignin encrustation of the cellulose microfibrils in the cell wall confers rigidity, and because of lignin less hydrophilic properties, it also influences the swelling characteristics of wood.
Figure 9 Scheme representation of possible bonds in lignin polymer.
The association among cellulose, hemicellulose and lignin needs to be considered. It is generally accepted that the less-ordered cellulose is linked to hemicellulose molecules through hydrogen bonds; hemicellulose is then linked to lignin molecules through
covalent bonds, acting like a sort of “glue” between cellulose and lignin (Figure 10).
Thanks to the presence of a lot of hydroxyl groups, hemicellulose molecules are the wood most hydrophilic compounds and represent the cell wall areas through which polar solvents can diffuse.
Figure 10 Scheme of the association between cellulose, hemicellulose and lignin. a) Transversal section; b) longitudinal section (from Nardi, 2006).
Substances with low molecular weight
The so called extractives are low molecular weight organic substances that can be extracted from wood using polar (e.g. acetone, water, ethanol) or apolar (e.g. toluene) solvents. Although if they represent only in a small percentage of wood cell walls (1.2%
of dry mass for hardwood, from 3.5% to 10% for softwood, the extractives influence colour, hygroscopicity, smell and resistance. In some species, they are toxic and play a role against the attack by bacteria, fungi and termites.
The extractives of conifers can be classified into three categories (Frengel, 1989):
1. terpenes and terpenoids (molecules are composed of units of isoprene, up to six grounds in the same molecule)
2. aliphatic saturated and unsaturated fatty acids, alkanes and fatty alcohols (e.g.
triglyceride, palmitic acid, stearic acid).
3. phenolic compounds (e.g.vaniline), lignans (e.g. pinoresinol, hinokiresinol) and stilbenes.
The mineral compounds of wood are entirely contained in the ash after combustion of organic matter. They represent the 0.1% dry weight for trees located in the temperate regions. The most abundant minerals are phosphorus, calcium, potassium and magnesium.
1.2.2 Wood properties
There is a strong relationship between the properties of wood and the properties of the particular tree that yielded it. For every tree species there is a range of density for the wood it yields. There is also a rough correlation between density of a wood and its strength (mechanical properties). For example, while mahogany is a medium-dense hardwood which is excellent for fine furniture crafting, balsa is light, making it useful for model building. The main features of some species of commercial importance are reported in Table 1.
Table 1 Features of some wood species in use for human artefacts (data from ottimari.agr.unifi.it;
COLOUR [g/cm3] DENSITY (for UL=12%) SHRINKAGE[%]
Ax=axial; Rad=radial; Tan=tangential; Vol=volumetric AXIAL COMPRESSION STRENGHT (for UL=12%) [MPa] FLEXION RESISTANCE (for UL=12%) [MPa] ELASTIC MODULUS [MPa] IMPREGNABILITY(1=very high; 5=verylow)
Abies alba Mil.
White 0,44 Ax:0,3 Rad:3,5 Tan:7,2 Vol:11
38 70 14500 Alburno: 2 Duramen:
Pinus sylvestris L.
white- yellowish Duramen rosate
0,55 Ax 0,4 Rad 4,1 Tan 8,3 Vol: 13
46 98 14000 Alburno: 1 Duramen:
Larix decidua Mill. Alburno
white- yellowish Duramen:
0,65 Rad: 3,4 Tan: 8,3 Vol:13,8
52 95 14300 Alburno: 2 Duramen: 4
Castanea sativa Mil.
Alburno white- yellowish Duramen:
0,57 Rad:0,3 Tan:6,6 Vol:11,2
52 110 11600 Alburno: 2 Duramen: 4
Populus alba L.
Alburno white- yellowish Duramen:
0,82 Ax:0,4 Rad:4,4 Tan:8,3 Vol:13,2
62 110 12800 Alburno: 1 Duramen: 4
Quercus robur L.
0,34 Rad:4,4 Tan:8.36 Vol:13,2
32 56 Alburno: 1
1.3 Wood degradation
When untreated wood is exposed to adverse conditions, it can degrade back to carbon dioxide and water through a series of chemical pathways. Fungi, termites, heat, humidity, ultraviolet energy, and chemicals can modify the performance properties of wood. Generally, it is common practice to distinguish between abiotic and botic degradation.
1.3.1 Abiotic degradation
When wood is exposed to outdoor climate, a complex combination of chemical, mechanical and energy factors contribute to what is described as a weathering. We tend to study each of these degradation chemistries as individual events but, in fact, they are all connected by five basic chemical processes: hydrolysis, oxidation, dehydration, reduction, and free radical cleavage (Comstock, 1984).
The chemical reactions involved lead to the degradation of both cellulose (and hemicellulose) and lignin. Cellulose degrades primarily by hydrolisis of glycosidic bonds and oxidation of the polymeric chains extremities; lignin is subjected to substitution reactions, oxidation and hydrolysis, and its reactivity is due to the benzylic, hydroxyl, carbonyl and carboxyl groups on its propanoidic chains and to the phenolic function and aromatic nucleus.
Water is one of the main factors of wood degradation.
Especially when wood is used outdoors, temperatuee and humidity variations cause changes of wood moisture content until new equilibrium conditions (EMC) are reached (Figure 11).
Wood hydroxyl groups, and especially those of hemicellulose, confer a strongly hydrophilic character to the cell walls. When wood is exposed to high relative humidity (RH), water molecules diffuse in the cell walls through formation of hydrogen bonds, resulting in wood swelling. When the cell wall saturation point is passed, water flows in the cell lumens as free water. This process is reversible and wood exposed to variable weather conditions will undergo cycles of shrinking and swelling that can cause cracks in the material.
Figure 11 Wood equilibrium moisture content [EMC%] related to the temperature and humidity [RH%] of the surrounding air (www.cas.purdue).
Sun radiations can even cause wood degradation. Wood is a good light absorber due to the presence of several chromophores, e.g. phenolic hydroxyl groups, aromatic skeleton, double bonds and carbonyl groups. The UV light component of sunlight, which acts in combination with moisture, temperature, and oxidative agents such as oxygen and/or ozone, depolymerise both lignin and cellulose (Hon, 1994, Evans, 1992).The oxidation of wood causes discoloration, followed by loss of gloss, roughening and checking, attributed to the formation of carbonyl, α-β-unsaturated systems in the cellulose and to the modification of the chromophores of lignin, capable of absorbing UV light in the range of 300–400 nm. It also causes an increase of susceptibility to other degradation phenomena such as acid and alkaline hydrolysis, both favored because influenced by the electronic effect of oxidized groups on C (6), C (3) and C (2).
Wood is also susceptible to acid or base attack (Campanella, 2007). Cellulose glycosidic bonds may be splitted by acid hydrolysis, which takes place even at relatively low
temperatures (homogeneous hydrolysis by H3P04 is usually carried out at 25°C) and proceeds through the protonation of the hemiacetal oxygen, the exit of the nucleophilic unit and the entry of water (Figure 12). Even a highly alkaline environment under high temperature conditions (above 150°C) can cause hydrolysis and degradation of the cellulosic structure. In this case, the hydroxyl deprotonation at C (2) creates a reactive nucleophilic specie (alkoxide ion) that attacks the anomeric carbon, thus causing the separation of the alcoholic fragment of the glycoside (Figure 13).
This hydrolytic cleavage can occur randomly, i.e. at every point in the chain. In alkaline environment, further degrading hydrolysis may occur even at temperatures below 100°C, known as peeling off: the reducing end (terminal glycose) of the cellulose molecule isomerizes, through the ene-diolic form, in the corresponding ketose, on which a 3- elimination reaction occurs; if it involves the C (4) position, the remaining part of the chain is removed (Figure 14), the residual ketose undergoes further transformation to isosaccarinic acid. The reaction is repeated on the new reducing ends of the chain and then degradation takes place with the detachment of a unit at a time, hence the name of the process (Campanella, 2007).
The hydrolytic processes cause a decrease of the cellulosic degree of polymerization and a consequent reduction of wood mechanical properties.
Lignin can be also subjected to basic attack due to its carboxylic groups and phenolic groups, that may participate in different reactions creating reactive radicalic, quinonic and anionic intermediates.
Figure 12 Acid hydrolisis of cellulose (Campanella, 2007).
Figure 13 Alkali hydrolisis of cellulose (from Campanella, 2007).
Figure 14 Cellulose dagradation by peeling off (from Campanella, 2007).
1.3.2 Biotic degradation
Wood can be degraded by a variety of organisms, causing aesthetic and/or mechanical decay.
The main organisms causing wood biological degradation are reported in Table 2.
Table 2 Main organisms causing wood biological decay (Shmidt, 2006).
Organism Mechanical damage Aesthetic damage
Coleoptera insects yes yes
Isoptera insects (thermites) yes yes
Basidiomycetes fungi yes yes
Chromogenic fungi no yes (non removable)
Soft rot fungi yes (superficial) yes
Molds no yes (removable)
Marine borers yes yes
Fungi are eukaryotic and carbon-heterotrophic (free from chlorophyll) organisms with chitin in the cell wall, reproduce asexually and/or sexually by non-flagellate spores; they can be unicellular or pluricellular, but the unicellular forms have a minor part to play in the colonization and decay of wood. Pluricellular fungi are filamentous: they are formed by hyphal filaments and colonize wood through the apical growth of hyphae.
They develop in wood if some environmental conditions are satisfied: depending on fungi and wood species, wood moisture content of about 20% or more and atmospheric temperature ranging from about 10°C to 40°C make wood susceptible to fungal attack.
Wood-stain fungi are highly pH sensitive, with pH values of highest growth depending on the specie; they usually grow best in slightly acidic substrates but can also do well in higher pH levels. Basidiomycetes, for example, have an optimum range of 4-6 (Schmidt, 2006) Also light is known to influence enzyme regulation in fungi and there are examples of increased activity of some enzymes and inhibition of others (Eaton, 1993).
Fungal chemistry of decay mainly consists of cell wall enzymatic degradation. More than 3000 wood degrading enzymes are described comprising both polysaccharide degraders (cellulases and hemicellulases) and lignin modifying enzymes.
Cellulose is depolymerized by three major classes of hydrolytic enzymes: endocellulases (Cx), exocellulases (C1) and β-glucosidase, generally acting synergically in a multi-step process. Endocellulases attack by hydrolysing non-cristalline regions and regions of less ordered crystalline cellulose thus opening up cellulose chains. The cellobiohydrolase (exocellulase) binds to the edges of the cellulose crystallite and cleave off cellobiose units from the non-reducing ends. In addition, it opens up various random points of the crystalline regions, instantaneously attacked by endocellulases. β-glucosidase converts cellobiose to glucose.
Oxidative enzymes (cellobiose oxidases and glucose oxidases) and oxidoreductive enzymes (cellobiose dehydrogenase) also participate in cellulose degradation. Cellobiose oxidases enzymes act on crystalline cellulose producing gluconic and cellobionic acids.
Action on the cellulose reducing-end groups would result in the production of acid groups and would open up the crystallite allowing endocellulase action.
Hemcellulose is degraded by hydrolytic enzymes (both exo- and endo-enzyme types); the
most diffuses among fungi are: xylanases (1,4-β-D) (that may be divided in those which cleave at L-arabinose branch points or those that cleave throughout the xylan polymer leaving xylobiosyl and xyloriosyl residues attached to the L-arabinofuranose), mannanases (1,4-β-D) and galactanases (1,3-β-D). The preferential ability of certain wood-decay fungi to attack different susceptible wood species may be related to hemicellulose composition (Schmidt, 2006).
Lignin degradation by white rot fungi is acheived by an oxidative radical mechanism involving a lignin peroxidase (ligninase) and hydrogen peroxide (generated during cellulose degradation by glucose oxidase) and by other phenol-oxidizing fungal activities.
The lignin-degrading activity of white rot fungi is characterized by the production of phenoloxidases, in particular the copper-containing enzyme called laccase. Some of the pathways attributed to the oxidation reactions of laccase on phenolic end-groups of lignin (Shimada, 1991) are reported.
Since the enzymes are too large to diffuse freely in the unaltered wall, it is now commonly accepted that non-enzymatic, low molecular weight metabolites (oxidative free-radicals) are also involved as precursors and/or co-agents with enzymatic degradation. The main non-enzymatic systems proposed involve Fe2+, H2O2, oxalic acid and the production of hydroxyl radicals (Schmidt, 1981).
Taxonomically, the fungal species responsible for wood decay belong to the subdivisions of Ascomycotina, Basidiomycotina and Deuteromycotina; as concerns decay modalities, wood decay fungi have been categorized, since 1874 in species causing brown rot and species causing white rot.
Brown rot is caused by Basidiomycetes which metabolize the carbohydrates cellulose and hemicelluloses of the woody cell wall by non-enzymatic and enzymatic action but leave the lignin almost unaltered. In fact, brown rot fungi don’t produce phenoloxidases: lignin degradation is limited to extensive demethoxylation of the aromatic portion with the loss of the propane side chain and the incorporation of molecular oxygen.
Brown rot fungi colonize wood via the rays and spread in the longitudinal tissue through pits and by means of microhyphae. They grow inside the cell lumina and there in close contact with the tertiary wall. The low-molecular agents and/or the cellulolytic enzymes penetrate through the relatively resistant tertiary wall (high lignin content) and diffuse
into the secondary wall, where they degrade the carbohydrates completely. Due to the rapid cellulose depolymerization, the dimensional stability and mechanical properties particularly decreases. During Serpula lacrymans attack, for example, a decreasing of the compression strength by 45% at only 10% mass loss is reported. Brown-rotted wood is reddish brown to dark brown in appearance due to the increase of relative lignin content.
At late stage of decay, especially in drying conditions, wood commonly shows deep cross-cracking due to shrinkage caused by the loss of carbohydrates in the wood cell wall. The residue of heavily decayed wood (mainly modified lignin) easily crumbles between the fingers to a fine powder.
Many brown rot fungi have a tendency to be potent acid producers and can cause a drop in pH of the growth medium. The acid substances produced are a variety of organic acids, notably oxalic acid. Particularly in later stages of decay, the highly lignified middle lamella/primary walls were observed to undergo attack. Also, the penetration of the wood cell wall by bore holes removes lignin in the process, all suggesting that low molecular weight lignin degrading agents and potentially even lignin degrading enzymes max occur in some brown-rot fungi, at least with localized activity (Goodell 2003).
Most brown-rot fungi affect conifers (Ryvarden 1993) and are usually uniformly distributed over the substrate.
The characteristics of the brown rot fungus Coniophora puteana are reported in Table 3.
White rot is caused by basidiomycetes and some genera of ascomycetes which not only metabolize cellulose and hemicelluloses but are also able to degrade lignin extensively due to the production of phenol-oxidases. They often cause the decay of lignin, hemicellulose and cellulose at the same time and similar rate (“simultaneous white rot fungi”), but some species degrade lignin and hemicellulose before the cellulose in the cell wall is attacked (“preferential white rot fungi”). They colonize the wood via ray parenchyma and vessels or resin canals (in softwoods) and grow principally in the wood cell lumina. Hyphal colonization from cell to cell in early decay may happen through the pit pores but, latterly, bore holes are produced and a gradual thinning of the wood cell wall around fungal hyphae is seen. The middle lamella is only finally dissolved in later stages of decay leading to a complete breakdown of the wood cell wall structure (Schmidt, 2006).
Table 3 Main features of the brown rot fungus Coniophora puteana (Shum.:Fr) P. Karsten.
Coniophora puteana (Shum.:Fr) P. Karsten
Domestic (buildings) and external.
Image from www. societe-mycologique-poitou.org Growth and decay conditions
Temperature: optimum: 23°C; range:3-35°C; survives in kilns at 50-65°C for several weeks. Moisture content: optimum: 50-60% (minimum in spruce sapwood:24%)
Wood species attacked
Mainly softwoods, sometimes hardwoods (e.g. oak)
Rate decay of wood
60% weight loss can be achieved in 12 weeks in soil block test on Scots pine sapwood
Notes The characterization of the cellulolytic enzyme system and of some mechanisms of wood degradation are reported in literature (Hyde; Lee et al. 2004).
Table 4 Main characteristics of the white rot fungus Trametes versicolor (L.:Fr.) Pilat.
Trametes versicolor (L.:Fr.) Pilat.
Wounded or dead standing trees, logs and stumps, rarely in buildings.
Image from Schmidt, 2006 Growth and decay conditions
Temperature: optimum: 30°C; maximum: 36°C;
moisture content: optimum: 40-45% or higher.
(minimum in spruce sapwood:24%).
Wood species attacked Mainly hardwoods, occasionally softwoods
Rate decay of wood
38% weight loss can be achieved in 16 weeks in agar block tests on beech (Fagus sylvatica L.)
Notes The decay by a simultaneous type of attack is described in literature (Schmidt, 2006).
White-rotted wood takes on a lightened bleached appearance; it may become rather fibrous along the grain due to the separation of wood cells along the middle lamellae and the surface becomes softened. The wood strength properties are reduced to a lesser extent than in brown-rotten wood, since at the same mass loss, lesser cellulose is consumed, and it does not come to cracking or cubical rot. In a very late stage of attack, a wood mass loss of 97% has been measured. Hardwoods are generally more susceptible to white rot than softwoods. The characteristics of the white rot fungus Trametes versicolor, whose type of attack has been object of many studies on the micromorphology of white rot, are reported in Table 4.
Wood-decay insects causing damage to timber and wooden artifacts can be referred to the taxonomic orders of Coleoptera (Anobiidae, Lyctidae, Bostrychidae, Cerambycidae, Curculionidae), Hymenoptera (Siricidae) and Isoptera (Rhinotermitidae and Kalotermitidae) (Chiappini, 2001).
Adults of Coleoptera and Hymenoptera generally depose their eggs on the wood surface;
the eggs open and, in the stage of larvae, penetrate the wood structure excavating galleries; inside wood larvae develop in pupae and finally in adults, that fly outside wood.
They attack mainly wood with moisture content of 7-15% (indoor structures) or >15%
(timber). As regards buildings, the attack is normally extended to the whole length of the wood structural elements and cause mechanical resistance diminution proportional to the section reduction.
Isoptera comprise Termites, social insects living in colonies. A termite colony is a complex community whose individuals have particular roles and functions concerning with either defence and protection of the nest against predators (“soldiers”), labour including foraging for food (“workers”) or reproduction to expand the existing colony or establish a new colony (“reproductives”). They usually make their nests in soils and extend into the wood by excavating tunnels and galleries, inflicting destruction
especially on timber used for constructional purpose both outdoors and inside buildings.
Their ability to destroy wood is due to the population of symbiotic bacteria, protozoa or enzymes in their gut which assist in the breakdown of ingested lignocellulosic food material (Goodell, 2003). The species of termites more diffused in the italian geographical region are the drywood termites Kalotermes flavicollis (Fabricius) and the subterranean Reticulitermes lucifugus (Rossi). Their main characteristics are reported in Table 5.
Table 5 Main features of the termites Kalotermes Reticulitermes (from Chiappini,2001).
(Drywood termites) Reticulitermes
(Subterranean termites) Image
Kalotermes flavicollis (Fabricius) Reticulitermes lucifugus (Rossi).
Occurrence Wounded or dead standing trees, buildings, ceilings, roofs, wooden artifacts, beams, frames.
Buildings (churches, libraries, archives) also in urban areas, ceilings, roofs, wooden artifacts, beams, frames, paper.
Wood attacked Springwood, especially with low humidity (drywood)
Wood characterized by high moisture content.
Growth and decay
Colonies, usually not larger than 1000-2000 individuals, make their nest inside wood.
Colonies, usually numerous (larger than 100000 individuals), make their nest on the soil or, sometimes, in empty spaces inside walls and door-frames. The system of unneling is employed to move upward without being exposed to the sunlight.
188.8.131.52 Wood durability against fungi and insects
Timber species differ markedly in performance when exposed to decay risks: the term
“natural durability” is used to express a wood species intrinsic resistance to defined xilofagous organisms. It is generally referred to the duramen (alburno is often easily degradable) and depends on chemical and physical characteristics of wood, such as density, nitrogen and starch content, lignin quantity and type and especially the presence of extractives (cyclic, aromatic or phenolic, produced as secondary metabolites via the shikimic acid pathway (hydrolysable tannins, lignans, coumarins, alkaloids), via mevalonicacid (terpenoids, steroids) or by combinations of these two pathways (stilbenes, flavonoids, condensed tannins).
The main characteristics of durability of some wood species used for human artefacts are reported in Table 6.
Table 6 Natural durability of some wood species. Scale of durability against fungi basidiomycetes (UNI EN 350/1): 1=Very durable, 2=Durable, 3=Moderately durable, 4=scarcely durable, 5=Non-durable; Scale of durability against insects (UNI EN 350/1): D=Durable, MD=Moderately durable, ND=Non-durable.
Wood specie Fungi basidiomycetes Hylotrupes bajulus Anobium punctatum Termites notes
Abies alba Mill. 4 ND ND ND
Pinus sylvestris 4 // ND ND
Larix decidua Mill. 3-4 ND ND ND
Castanea sativa Mill. 2 // ND ND Alburno Hesp.
Fagus sylvatica L. 5 // ND ND Hesp.
Populus canescens sm 5 // ND ND Hesp.
Juglans regia L 3 // ND ND Hesp,
Quercus robur L. 2 // ND MD Alburno Lyctus, Hesp.
1.4 Treatments for the improvement of wood properties
Treatments for wood protection and enhancing of properties have been known for almost as long as it has been in use (Mahltig, 2008). Treatments aim especially at the improvement of mechanical resistance, water resistance (dimensional stability of wood), fire resistance and UV protection.
1.4.1 Surface Coatings and penetrating treatments
The most common method of protecting wood from weathering and photodegradation is the use of a wide range of coatings such as paints, varnishes, stains and water repellents (Williams, 1999).
In fact, surface coatings, e.g. varnishes, waxes or natural oils such as olive oil, have been applied since ancient times.
Wood coatings are generally classed as either film-forming or penetrating. Film-forming treatments, such as paints, contain pigments that screen wood from solar radiation and, because they form a barrier over the wood surface, they also prevent surface wetting and erosion. Nevertheless, their main drawback is the loss of adhesion during weathering due to failure of the underlying wood (Adebahr, 2000; Fauchadour, 2005). They are also scarcely effective in controlling wood dimensional changes.
Penetrating treatments typically contain a hydrophobic component such as waxes, natural oils or resins.
The formation of a hydrophobic coating raises the contact angle of the treated wood preventing water from being readily taken up by the surface or sub-surface capillaries.
This reduces moisture absorption and imparts a certain degree of dimensional stability to wood (Evans, 2009).
Additives are often added to coating products to enhance wood stability to solar radiation. For examples, stains containing pigments partially obscure the wood surface, and hence reduce the amount of light reaching the wood. A more efficient protection of wood can be achieved by reflecting or harmlessly absorbing UV radiations, the main responsible for photodegradation. Stains containing UV reflectors (from 0.01 to 0.15 μm particles, able to scatter UV light while having little effect on visible light, such as micronised titanium dioxide or micronised zinc and cerium oxides) or UV absorbers (a
wide range of organic molecules, including benzophenone, benzotriazole and triazine, whose UV absorbance is determined by the chromoforic group, whereas the volatility, polarity and resistance to leaching are controlled by molecular weight and nature of substituent groups) have also been used.
Flame retardant additives used in the past are: chlorinated and brominated biphenyls and diphenyls, carrying high environmental and health risks; boric acid, soluble zinc, phosphorous and metal salts, whose main disadvantage is the low leaching resistance when in contact with water. (Mahltig, 2008).
1.4.2 Modification of wood
Since the abiotic and biotic decays are related to the molecular properties of the constituents of wood, it is possible to eliminate, or at least limit them by chemically modifying the structure of lignocellulosic polymers. Wood properties can be improved by chemical modifications, generally obtained by covalently bonding chemicals to the polymeric constituents of wood and, in certain cases, by bulking the cell wall (Mahltig, 2008). During recent years the numbers of methods and procedures developed to modify wood have increased and a wide variety of compounds have been employed for wood modification including anhydrides, acid chlorides, carboxylic acid, isocyanates, aldehydes, alkyl chlorides, lactones, nitriles, and epoxides (Militz, 1997; Norimoto, 2001), aiming at enhancing wood durability, dimensional stability, strength and hardness, weathering performance and flame resistance (Donath, 2004). In this way, new wood products can be made which differ absolutely in their technological properties from the original wood.
The most effective technologies used are heat treatment, acetylation, furfurylation, treatments with silica, silicones and silanes and treatments with chitosans. There are still many questions concerning the active principles, effectiveness, costs and optimization of these single technologies (Mahltig, 2008).
Several processes to thermally treat wood have been commercialised in Europe in the past decade and are currently used in many indoor and outdoor applications. Various thermal processes have been developed, consisting of wood treatments at elevated temperatures (160-240°C) in conditions of low wood moisture content (by means of
drying steps) and low oxygen present (under-vacuum or nitrogen atmosphere conditions).
Linseed oil is used in the OHT (oil heat treatment) process (Germany) as a drying medium and to improve heat flow into the timber; at the same time, the oxygen level in the vessel is low due to the oil (Shultz, 2008). Chemical changes due to thermal treatments to the wood structural polymers, such as increase of the relative amount of crystalline cellulose and lignin bond rearrangements with subsequent formation of a more condensed structure, lead to dimensional stability improvement, decrease hygroscopicity and physical/strength alteration.
Acetylation consists of the substitution of wood hydroxyl groups, responsible for the interaction of wood with the environmental water, with acetyl hydrophobic groups, reducing in this way the moisture content exchange (EMC) and consequently the swelling and shrinkage of wood to a great extent.
Modification of wood with furfuryl alcohol-resins is called furfurylation. Furfuryl alcohol polymerize in situ in presence of an acid catalyst (cyclic carboxylic anhydrides are often used) and reacts with the cell wall components (especially with lignin) leading to an improvement of dimensional stability, anti-shrinkage efficiency and resistance to alkali and acids.
Polyethylene glycol or wood plastic composites were also employed, however these treatments often cause high gain of weight and related drawbacks to the advantages of wood (Okawa, 2002).
Applications of nanotechnology to wood had been performed in recent years, also for the conservation and restoration of the world’s cultural heritage: the use of nanoparticles of calcium and magnesium hydroxide and carbonate to restore and protect wall paints and to de-acidify paper and wood is reported (Baglioni, 2006). In particular, wood treatments based on nanoparticulate silica sols (“nanosols”) have been studied in the last decades. Nanosols consists of transparent, nano-sized (usually les than 50nm) dispersions of inorganic particles in either water or mixtures of organic liquids, applied as coatings of the wood surface or for impregnation of the whole wood body.
Among the range of wood modifiers, also many types of silicon compounds have been
used (Kartal, 2007; Mai, 2004; Saka, 2001), obtaining improvements in certain physical properties. The silification of wood has been inspired from nature: in the Petrified Forest National Park, Arizona, wood became fossilised and its organic matter was penetrated by minerals (mostly silicate) yet the original structure is still retained after more than 200million years (Mahltig, 2008). Since the 1800s sodium silicate-based treatments were applied trying to mimic the natural process of silification of wood.
A review about the modification of wood with silicon compounds has been recently published (Mai, 2004).
Silica modifications of wood recently studied are mainly based on:
- silica nanosols prepared from aqueous sodium silicate - commercially available products containing colloidal SiO2
- silicon alkoxide precursors
Due to their high surface-to-volume ratio, inorganic nanosol particles are metastable.
Thus, during the application to wood and subsequent drying, these materials condense into an inorganic three-dimensional xerogel network, modifying the substrate properties.
Inorganic nanosols have been applied to wood in order to improve its properties and for consolidation purposes. In fact, cracks can appear on wood due to swelling and shrinking processes caused by changing temperature and climate and by the natural movement of the wood material itself: silica treatments can improve wood mechanical characteristics (Sèbe, 2004; Mai, 2004) as demonstrated by increased Brinell hardness. The introduction of organic additives with an affinity to wood but which don’t hinder penetration into the wooden structure makes it possible to achieve a maximum degree of consolidation (Böttcher, 2000); recent applications for restoring and preserving wooden cultural artefacts are reported (Mahltig, 2008).
Resistance of wood treated with silica compounds to liquid water sorption (Temiz, 2006) to photochemical degradation (Temiz, 2004; Temiz, 2006), to combustion (Saka, 1997;
Yamaguchi, 2003), especially if in combination with boron (Furuno, 1992; Furuno, 1993) and to swelling (Ogiso, 1994) have been reported. In a recent report, many ways in which the properties of wood might be improved by application of silica and other inorganic nanosols have been reviewed (Mahltig, 2008).
The presence of silica in the cell walls, rather than in the lumina, depends on wood moisture content. This can influence the material final properties: in general, the
increase of durability, dimensional stability and UV-VIS radiation resistance are due to silica compounds deposited onto the cell wall, whereas the presence of chemical compounds into the cell lumen can influence hardness and flame resistance, but don’t make any contribution to decreased water absorption (Saka, 1992; Mai, 2004). The addiction of hydrophobic, fire resistant, coloured or UV-protective additives is reported to improve other important properties of practical interest (Table 7).
Table 7 Additives to silica treatments for the improvement of wood physical/chemical properties (Malthing, 2008).
184.108.40.206 Silica modification with alkoxysilanes
The most convenient method for modify wood is to impregnate the cell wall with alkoxy monomers which are then allowed to polymerise in situ.
Polymerisation of the alkoxysilanes monomers can be achieved by the sol-gel process, i.e. via condensation of the silanol Si-OH groups to form siloxane bonds after hydrolysis of the alkoxy groups. (Brinker, 1990; Brebner, 1985). (Figure 15).
The so formed siloxane polymers can penetrate into the wood texture and interact, mainly via hydrogen bonds, with the wood biopolymers of the cell walls (Schneider, 1985). The possible formation of Si-O-C covalent bonds, by reaction between the silanol groups and the hydroxyl groups of cell wall polymers (transesterification), has been also suggested (Sébe, 2001); nevertheless, this is considered less favoured with respect to the formation of H-bonds by another research group (Ogiso, 1994). The siloxane materials can polymerize both onto the cell walls and inside the lumina. In the last case they behave as simple filling materials exhibiting a sort of barrier effect. In the first case, the presence of silica in the cell walls, rather than in the lumina, strongly influences the resistence of the wood by modifying its physico-chemical characteristics.
Wood property Additive
Hydrophobic Long-chained alkylsilanes
Colored Inorganic color pigments Natural or synthetic organic dyes
UV-protective Organic UV absorbers
Inorganic pigments like TiO2, ZnO
SOL-GEL PROCESS – ALKOXYSILANES METHOD
Figure 15 Scheme of the sol-gel process with its hydrolysis and condensation reactions.
In recent reports, many ways in which the properties of wood might be improved by application of silica and other inorganic nanosols have been reviewed: various methods of treatment, from superficial coating, to impregnation under vacuum, and various silane precursors have been tested and compared (Mahltig, 2009, Tingaut, 2005; Tingaut, 2006; Sèbe, 2004)).
Improvements of physical properties of wood through modification with alkoxysilanes are reported. They span from water repellency (De Vetter, 2010), resistance to liquid water sorption (Brebner, 1985), to photochemical degradation and artificial weathering (Tshabalala, 2003; Donath, 2007), to combustion (Saka, 1997) especially if in combination with boron compounds (Marney, 2008) and to shrinkage (Saka, 1992;
solution of precursors sol (colloid) gel xerogel drying
gelation hydrolysis and
1.5 Preservation of wood from biotic decay
Wood preservation includes physical or chemical treatments aiming at hinibiting the activity and viability of wood-degrading organisms (remedial treatments) or applied on wood in order to prevent biological attack (preventive treatments).
The landscape of both remedial and preventive preservative treatments has changed drastically in the last few years (Manning, 1997; Hughes, 2004; Lack, 2008).
In 1998 the European Directive on the Biocidal Products (98/8/EC) listed different biocidal product types including, among them, wood preservatives (Product Type 8).
According to Article 24 (1) of Directive, Member States have to take the necessary arrangements to monitor whether biocidal products placed on the market comply with some enounced requirements: the Biocidal Products Directive BPD 98/8/EC (1998) came into force in September 2006 and approximately 50% of biocides for wood preservation were removed from the market due to their toxicity for human body and for the environment.
The list of banned biocidal products is reported in the Official Journal of the European Union, Commission Regulation (EC) No 1451/2007 of 4 December 2007.
1.5.1 Remedial treatments
Since the last few years the main chemical remedial treatments against wood biotic degradation have consisted of the application on wood of preservative formulations whose main active ingredients were: mercury, copper, arsenic or other metal and organometal compounds, boron compounds phenolic and trisubstituted tin compounds, thiazoles, polyoxins, petroleum and tar oils, alkylammonium compounds and N- trichloromethythio or phithalimide biocides (Schultz, 2008).
Their modes of action on fungi include inhibition of respiration (copper and arsenic compounds, phenolic compounds, thiazoles such as isothiazolones), inhibition of biosynthetic reactions in cells such as chitin synthesis (polyoxins) and lipid synthesis (imidazoles, pyrimidines, triazoles), inhibition of cell division (benzimidazole derivatives) and non-specific inhibition of several enzymatic processes at the same time (quaternary ammonium compounds, mercury-based compounds, N-trichloromethylthio or phithalimide compounds).
The main active ingredients of preservative formulations to control attack by insects are included in the categories of pyretroids, organophosphorous compounds, carbamates cyclodienes and gamma-HCH. Pyrethroids are mainly used as insecticidal components in many organic-solvent wood preservative formulations and as soil treatments against termite infestations. All these insecticides exert an effect on the insect nervous system by interfering with axonal transmission (pyrethroids), inhibiting acetylcholinesterase activity (organophosphorous compounds, carbamates) or causing excessive release of acetylcholine (gamma-HCH).
Most of the active principles reported above have been banned by the European Community because of their persistence in the environment and high toxicity for human body. Nowadays some copper compounds, quaternary ammonium compounds and boron compounds are admitted, under specific concentration levels. Most of these products have been also used for preventive purposes and will be discussed in the following section.
Copper compounds have been used as fungicides over a century and copper sulphate or other salts have been applied against fungi causing diseases in agricultural crops as well as decay in wood but they are scarcely resistant to water leaching (Shultz, 2008). Other compounds have also been used in the past (e.g. copper oxide, copper naphthenate, copper-8-hydroxyquinoline complex, copper chelates with dialkyldithiocarbammates).
The mode of action proposed are the non-specific denaturation of proteins and enzymes, due to the Cu2+ affinity for thiol groups in the fungal cell, and the inhibition of respiration due to Cu2+ interference with the activity of conversion of pyruvate to acetyl coenzyme A.
Alkylammonium compounds, especially quaternary and tertiary amine salts, are general biocides that inhibit the cell respiratory activity and affect the semi-permeable membrane causing leakage of cell constituents. Tertiary amines and tertiary amine salts are thought to inhibit extra-cellular hydrolytic enzymes. They are also used as bactericides and surfactants because they are cheap; the efficacy of the addiction of inorganic copper to quaternary ammonium compounds against wood decay fungi and termites has been proved (Tsunoda, 1987; Hwang, 2007).